THE HEVI-SAND PROCESSIs this new technology a good reason to consider changing foundry chromitesand quality assurance parameters?SynopsisFoundry grade chromite sand production methods and acceptance specifications havechanged little in the last 50 years. This paper reviews the old, the existing, and thenew “Hevi-Sand Process” used to produce foundry chromite sand. The advent of newmining and processing technology , coupled with changes over the years in foundrypractices and procedures, suggests that new and standardized criteria for specifyingand testing of Hevi-sand processes products, (foundry chromite sands), is long overdue. This paper is therefore presented as a discussion document for change.The vast majority of chromite sand used in foundries comes from South Africa. Whilethere are large chrome ore deposits in other regions, the type of formation, crystal sizeand impurities, result in most instances, in undesirable foundry properties. The rest ofthis paper therefore only considers foundry chromite sands from South Africa.The area shown in fig1 is the Bushveld complex which contains among other thingsthe worlds largest chrome ore deposits. These deposits were formed throughprecipitation, as an underground magma lake cooled, and have been laid down asseams of variable quality and thickness, created by each change in the conditionswithin the magma lake. Subsequent earth movements have twisted the seams so thatin some places they are visible on the surface and in others are inaccessible at anyreasonable cost.
The seams have been classified into three main groups the upper groups, UG’s, themiddle groups, MG’s and the lower groups LG’s . Through reasons of mine-abilityand analysis, the UG’s are primarily mined for platinum group minerals, the MG’s forlower grade met grades, ferro- chrome, and the LG’s for high grade ferro-chrome,chemical grade and foundry sands. (see fig 2)South African Chrome Mining and ProcessingHistorically and up until 2008, most of the mining has been carried out by largemining houses that are either producing ferro-chrome or servicing ferro-chromeproducers. Foundry Sand has always been very much a by-product business ie lessthan 3% of the mined production ends up as foundry sand.Typically from 100 tons of mined ore, 33 tons would be Lumpy 44%Cr2O3, 33 tonssmall lumpy 42%Cr2O3, and 33 tons fines 35%Cr2O3. The lumps are fed straight tothe smelter for conversion into ferro- chrome, leaving the fines as a problem productdue to its low chrome content and high silicates contents. This material is traditionallycrushed and processed via “Humphrey spirals” (see fig3) to wash and concentrate it,into a useable product. (Humphrey spirals were developed in the USA during theSecond World War). Fig 3 Humphrey Spirals
This concentration usually results in three or four streams of product dependent on theconfiguration of the plant. For the 33 tons going into the plant, typically you wouldget 18tons of Met-grade 42% chrome, 9tons Chem.-grade, 3tons foundry grade and6tons of waste. See fig4 typical Chrome ROM and spiral processing plant layout Fig 4.Spiral plants work well with consistent feedstock , and work essential by pumping aslurry (water + chrome ore) to the top of spiral towers from where it runs downthrough the spirals and is concentrated based on particle mass / velocity by means ofweirs and diverters. It is effectively mechanised panning for gold.There are a number of obvious drawbacks with this system; variations in feedstock,slurry density, pump pressure, agglomerated fines, etc all make control very difficult.
It also requires large quantities of clean water, in what is a very arid area of RSAresulting in the need to recycle as much water as possible. When all these variablesare added together, the result is variable product quality.A new technology a new ideaIn the summer of 2004, price and availability of foundry chromite was becoming anissue. The commodity boom started to create a ferro-chrome shortage and thereforemost of the large mining houses concentrated on converting as much chrome ore toferro chrome as possible, to avoid letting down there core business, ie steel making,which in turn reduced availability and often the quality of foundry sand, which in turnpushed prices up.Amcol as a long term supplier to the foundry industry decided therefore, to investigatehow we could solve our supply and raw material quality problems. As we progress werealized that because of, history, concentration on core market, internal expertise andcommercial pressure, that none of the existing suppliers had any mining operationswhich focussed solely on foundry sand. Indeed the foundry Sand being produced wasas a result of a need to add some value to the fines, which are produced during mining/ processing operations to feed there ferro-chrome smelters. We decided therefore thatwe would concentrate our efforts solely on foundry sands and at the same time try todevelop a technology which maximised foundry sand yield, reduced waste andreduced the environmental impact of the process. Which concurrently reduced asmany variables as possible from the process, resulting in a range of products whichcould be tailor made to improved overall foundry Sand and more importantly castingquality.The “HS Process” was born through a mixture of our own internal researchlaboratory, external laboratory work, and discussion with some of the leadingprocessing companies in the world. As we progressed we came to understand theprocess requirements and the limitations of the existing spiral techniques. Weconcluded that with the right ore body, good liberation, and high technologyseparation, we could convert in excess of 65% of the mined ore body into veryconsistent high quality foundry sand, while at the same time reducing waterconsumption by at least 80%.The information, pictures and figures below (fig5-10) show some important aspectsinvolved in processing chrome ore. Fig 5. Chrome mining operations at Bathlako
Fig 6. Chrome ROM Crushing and ScreeningFig 7.Hard lumpy chrome ore Fig 8. Small Lumpy Chrome ore Fig 9. Washed and crushed chrome ore prior to processing
FIG 10. Crushed and washed chrome ore, note the liberated opaque silicates but also those silicates still attached to the grains. The chart below, (Fig11.) shows the assay of crushed unwashed lumpy ore and showsthat the majority of the, contaminates (silicates), are held either within agglomeratesie particles above 600micron or as fines. SiO 2 Cr 2 O 3 Fe O Grade Recovery Grade Grade Recovery Product Cumulative we ight fraction (%) (%) (%) (%) Recovery (%) (%) (%) Cr% Si% Recovery % Cr % Si % Primary -300 +212 Sinks 10.13 0.51 0.72 46.87 11.54 25.20 11.26 10.13 474.7931 5.1663 10.13 474.7931 5.1663 Primary -425 +300 Sinks 20.62 0.59 1.68 46.83 23.48 25.08 22.81 10.49 491.2467 6.1891 10.49 491.2467 6.1891 Primary -600 +425 Sinks 28.45 0.63 2.48 46.78 32.37 25.01 31.38 7.83 366.2874 4.9329 7.83 366.2874 4.9329 Secondary -600 +425 Sinks 32.76 0.67 3.05 46.78 37.26 24.97 36.08 4.31 201.6218 2.8877 4.31 201.6218 2.8877 Secondary -425 +300 Sinks 35.96 0.70 3.51 46.77 40.89 24.94 39.57 3.2 149.664 2.24 3.2 149.664 2.24 Primary -212 + 150 Sinks 44.44 0.79 4.88 46.70 50.47 24.99 48.98 8.48 396.016 6.6992 8.48 396.016 6.6992 Secondary -300 +212 Sinks 46.94 0.82 5.37 46.67 53.27 24.98 51.71 2.5 116.675 2.05 2.5 116.675 2.05 Primary -150 +106 Sinks 52.66 0.91 6.62 46.60 59.67 24.97 58.00 5.72 266.552 5.2052 5.72 266.552 5.2052 Secondary -212 + 150 Sinks 55.12 0.97 7.46 46.55 62.39 24.95 60.66 2.46 114.513 2.3862 2.46 114.513 2.3862 Secondary -150 +106 Sinks 57.32 1.06 8.44 46.47 64.77 24.93 63.02 2.2 102.234 2.332 2.2 102.234 2.332 Primary -300 +212 Floats 59.62 1.26 10.40 46.30 67.12 24.85 65.34 2.3 106.49 2.898 2.3 106.49 2.898 Primary-425 +300 Floats 62.13 1.52 13.11 46.07 69.60 24.74 67.80 2.51 115.6357 3.8152 2.51 115.6357 3.8152 Primary -106 71.05 2.44 24.10 45.22 78.11 24.36 76.32 8.92 Throw Away403.3624 21.7648 Primary -212 + 150 Floats 73.23 2.67 27.17 45.01 80.14 24.26 78.35 2.18 98.1218 5.8206 2.18 98.1218 5.8206 Primary -600 +425 Floats 76.13 2.99 31.63 44.73 82.80 24.14 81.05 2.9 129.717 8.671 2.9 129.717 8.671 Secondary -300 +212 Floats 79.26 3.47 38.24 44.32 85.42 23.97 83.82 3.13 2 Throw 3.13 138.7216 10.8611 Secondary -212 + 150 Floats 81.61 3.84 43.52 44.01 87.34 23.85 85.85 2.35 2 Throw 2.35 103.4235 9.024 Secondary -106 89.28 4.91 60.87 43.07 93.51 23.46 92.36 7.67 Throw Away Secondary -150 +106 Floats 90.99 5.14 65.02 42.87 94.85 23.37 93.80 1.71 2 Throw 1.71 73.3077 8.7894 Secondary +600 um 92.12 5.30 67.85 42.74 95.73 23.32 94.75 1.13 Throw Away 1.13 48.2962 5.989 Primary -150 +106 Floats 93.02 5.48 70.83 42.57 96.28 23.24 95.33 0.9 38.313 4.932 0.9 38.313 4.932 Secondary -425 +300 Floats 96.52 6.18 82.85 41.99 98.53 23.01 97.94 3.5 2 Throw 3.5 146.965 21.63 Secondary -600 +425 Floats 100.00 7.20 100.00 41.13 100.00 22.67 100.00 3.48 2 Throw 3.48 143.1324 25.056 22.97 3571.243 87.9902 3821.727 147.5749 afs54 77.03 46.36171 1.142285 83.41 45.81857 1.769271 Resulting analysis if throw away Resulting analysis if only all fines and float of secondary throw away fines materialWe therefore concluded that crushing and sizing along with liberation must becontrolled to maximise yield. When we looked at existing plants, most producers wereusing either Ball or rod mills to bring there spirals plant fines feed to grain size. Whilethis is of little importance when producing met grade smelter feedstock. The problemwith this approach to produce foundry sand is that it is akin to taking a sledge hammerto crack a nut and while reasonably effective at getting down to grain size andliberation levels it damages a lot of crystals and resulted in a lot of waste fines. In
some cases in excess of 35% of the feed is lost. Where as the calculable waste shouldbe less than 10%.After much discussion and trial work with various mill manufacturers we eventuallygot equipment from a USA manufacturer which could achieve impact liberation andsizing with little chrome crystal damage, (see fig 12). Fig 12. High level of liberation with little Crystal damage, utilizing controlled impact.Having achieved a significant improvement in liberation we then considered how toreduce water consumption and avoid the control difficulties surrounding the operationof conventional spiral plants. After many trials and brain storming sessions wedecided to concentrate on a wash process followed by dry separation. This resulted invarious trials etc with some of the equipment shown in fig13. These are rare earthmagnets, electrostatic separators and density separators. Fig 13.
The work resulted in our utilizing a mixture of fluidization, air classification, rare earth magnets and electrostatic separation and grain size classification. By combining these technologies we managed to achieve an 85% yield of saleable product through the process which also allowed us to produce multiple Hevi-Sand sizes without increasing impurities. As can be seen in the example Qemscan 180micron(fig14.) Fig 14 Qemscan data showing very low impurity levels.(green represents Cr) The Data below (fig 15.) shows how the HS Process from the initial pilot plant resulted in some interesting outcomes regarding chemical analysis, acid demand, size distribution and the resultant performance in this case with Alkyd type resin.Sieve Tests ASTM Sieve No 6 12 20 30 40 50 70 100 140 200 270 Pan AFS NoCurrent Material 0 0 0.187 3.462 21.557 42.062 27.473 5.125 0.118 0.016 0 0 41.5Hevi-Sand Tested Inhouse 0 0 0.06 3.049 19.241 30.862 27.019 13.912 4.95 0.871 0.036 0 48.2Hevi-SandTested Externally 0 0 0.11 3.12 20.21 34.02 28.05 12.17 1.93 0.06 0 0 44.9Acid Demand PH3 PH4 PH5Current Material 8.1 5.2 3.8Hevi-Sand 4 2.2 1.8Turbidity ppmCurrent Material 320Hevi-Sand >200Chemical Analysis Cr2O3 SiO2 CaO FeO LOI MoistureCurrent Material 45.80% 1.30% 0.53% N/A -0.85% 0.04%Hevi-SandTested Inhouse 47.90% 0.74% 0.39% 25.9 -0.78% 0.05%Hevi-Sand Tested Externally 48.23% 0.92% 0.43% N/A -0.80% 0.06%Tensile TestsTests done with 1.5% DYF-1 Alkaline Phenloic Resin, 25% DYG-4 Alkaline Phenolic Hardener at 24oC and 63% HumidityResults are in MPa after 24hrs Test 1 Test 2 Test 3 Test 4 Test 5 Test 6 AverageCurrent Material 0.643 0.999 0.854 1.024 1.055 0.665 0.873Volclay Hevi-Sand 1.222 1.352 1.451 1.086 0.922 1.207 (38% Increase in Tensile Strength compared to their existing material) Fig 15. As we have refined the HS Process, we are now producing product which typically contains fewer impurities ie assaying typically >48.0% Cr and <0.6 SiO2.
Furthermore, environmentally the process results in a 70% reduction in waterconsumption and waste, along with a 50% reduction in power, when compared to atraditional spiral plant.Given the above it drove us to try and understand more clearly how supply, time, andfoundries practical experience, had driven there understanding of and coloured, howthey defined good or bad chromite sand.Why do foundries use chromite sand?Chromite has a number of interesting properties useful to foundries -: 1. Linear Expansion (fig16.) chromite helps to stabalize predictable internal and external casting dimensions, while minimising the occurrence of veining. As can be seen Silica sand under goes a phase change at around 550oC which can lead to a number of casting problems. Thermal Expansion of Sand Silica Expansion 2 % linear Olivine 1 Chromite 0 Carbon Zircon 0 0 0 0 00 00 20 40 60 80 10 12 Degrees C Fig 15. 2. Heat abstraction (Fig 16,) on large castings in particular quality can be significantly improved if, as the mould is filled a solidifying skin is created as the metal rises up the mould face. Chromites high heat abstraction rate increases the thickness of the solidified skin, reducing the risk of it being washed away allowing faster filling times and rsing speeds. This high heat abstraction rate also aids in inhibiting penetration and burn on defects. FREEZING TIME SOLIDIFICATION 150mm SPHERE, (MIN) TIMES REF. TO SILICA SAND COPPER CHILL 4.2 .24 STEEL CHILL 4.3 .25 GRAPHITE MOLD 5.1 .30 CHROMITE BOND 13.4 .79
ZIRCON BONDED 13.8 .82 OLIVINE BONDED 15.8 .93 CHAMOTTE BOND 17.0 1.00 Fig 16. Other Hevi-Sand casting benefits 1. High fusion point 1850c, making in particular, core removal easier and improving cleanliness of feeder necks reducing the risk of the cutting flame being deflected into the casting. 2. It is chemically basic PH 6.5-7.5 making it less prone to, being wetted by steel, and slag reactions, when coupled with points 1-2-3 reducing penetration and burn on defects. 3. It can be used with all modern binder systems unlike olivine for example. 4. It does not react with manganese steels as does silica sand. 5. It has high permeability when properly vented reducing core temperatures and gas defects 6. It is reclaimable.Foundry problems with current supplyMost of the chromite sand used in foundries, is used in conjunction with resin bindersystems. Many of these systems rely on high efficiency mixers with low additionslevels, typically; resin 0.8% + an acid catalyst 0.125%. Therefore small variations insand quality can have a significant effect on these small additions and on the resultantmoulding sand properties. 1. Changes in acid demand / PH caused by poor water quality during sand processing, or high levels of alkaline impurities (silicates), can cause the resin not to harden properly, or too late, or too soon (if the sand quality improves over the norm). All of which are detrimental to foundries and ultimatelt casting quality. 2. Changes in Turbidity as above, but also increased incidence of double skin defects, ( see paper “Chromite Double Skin Defect on Heavy-Section Steel Castings” by same author). 3. Dust and segregation, caused by poor packaging, storage silo design , incomplete liberation, results in nuisance dust, variable sand curing times, and increased resin requirements.The problems above can increase resin costs, result in moulds being scrapped, or addfour months to the fettling and inspection time of large castings.It is therefore no surprise, that, foundries take chromite sand quality seriously, and testand specify some or all of the following parameters. 1. Chemical Analysis 2. Acid Demand at PH 5, PH 4, PH 3. 3. PH 4. Turbidity 5. Loss on Ignition
6. Afs. Number 7. Sieve analysis distribution. 8. FinesWe were surprised therefore when we started to collate worldwide foundry purchasespecifications, as part of our HS Process project objective, to decide what foundrieswould consider to be the ultimate specification. We found that there was a wide rangeand many variations in the test methods employed. Fig 17, shows some of thesefoundry purchase specifications.Typical foundry chromite order specificationsCr% FeO% SiO2% CaO% Turbidity AFS fines LOI PH Acid demand, ph 3, ph4, ph5>46% <29% <1% <0.5% <250ppm NA <1% NA <8.5 10ml, 6ml 4ml>45% <29% <1% <0.5% NA 50 <5% NA NA NA>44% <25% <4% NA NA 42 NA NA NA NA>44% <29% <4% <1.0% <400ppm 50 NA 0.5% NA NA>46% <25% <0.6% <0.4% <150ppm 48-52 <1% 0.1% <8.0 8ml 4.5ml 2.5ml>46% <26% <0.6% <0.4% <250ppm 60-70 <1% 0.1% <8.0 8ml 4.5ml 2.5ml Fig 17.It is important to note that what is reported as Si02 is not actually Si02 but a range oflow melting point silicates including enstatite , anorthite, and phlogopite.As you will see the range of specifications encompass nearly everything which couldbe described as chromite sand. In some cases met grade would meet the purchasespecification, which can often explain the variable casting results foundriesexperience. From further investigation it seems these specs have been developedbased on either, out dated information or by what has been available in the localmarket place, coupled with specification modifications, based on historic productquality problems. These problems were resolved via adjustments in AFS number orfines content, rather than addressing the fundamental realities of producing and usingthe product. It was also clear from our own experience and talking to foundry usersthat there had been many quality arguments over the years with suppliers, which hadoften turned out to be caused by differences in test methods. We therefore decide weshould start to compare the various test methods.Test MethodsChemical analysisMany foundries do not have equipment to test the chemical composition of chromitesand but the majority of those that do use XRF. One might think that this veryexpensive computer controlled method of analysis would produce very accurate andreproducible results. However, the calibration control program being used on the XRFmust be tailored to measure the high levels of chrome, iron, aluminium oxide andmagnesium typically seen in chromite sands. The correct chromite standards need tobe used for calibration to ensure accuracy in the desired ranges for each element. Forexample SARM 9 is a certified chromite standard from the critical zone of SouthAfrica’s Bushveld complex where much of the world’s foundry chromite sand issourced, it is a low silicate chromite and represents a very good standard to form acalibration around, as opposed to a high silica chromite standard from Kazakhstan orthe like. The XRF instrument prepares a standard curve for each element based on
certified standards; the instrument quantifies the fluorescent counts generated afterhitting the sample with x-rays at a given angle, the counts are then tied back to thecertified value of the standard (this is a very simplified explanation, more detailedinformation on XRF theory may be found by contacting Panalytical Instruments. Thevalues or counts are depended on sample preparation and sample matrix (you may getdifferent counts measuring Calcium in bentonite as opposed to Calcium in chromeore). The values for all the elements analyzed are added up into a sum, in fig 17.below, SARM 9 has a sum of 98.5 meaning if you analyzed the specified elementsyou should be analyzing 98.2% of that material, the remaining amount is composed oftrace elements not measured. Even using the same standards, differences can arisefrom how the standard curve is set up (which points are included, which areconsidered outliers etc). Fig 18 shows two chromite calibrations using the same set ofchromite standards while chromite calibration 2 gives preference to data points fromSouth African Chromite standards; calibration 1 treats data points from all standardswith equal importance.Most certified samples are ball milled resulting in a very fine particle size which isadvantageous for XRF analysis since it helps to ensure homogenous distribution of allthe phases in a given sample, some sample preparations even include preparing afused glass sample to provide an ideal sample matrix for the XRF to read, howeverthis preparation is more expensive than traditional “pressed powder” samplepreparations as it requires additional equipment and reagents. Typically chromite sandto be analyzed in a laboratory setting is not ball milled and in most cases, due to thehigh hardness, grinding of the chromite proves to be difficult unless the rightequipment is used. Coarsely ground samples will have low sums on the XRFinstrument which can skew results in either direction. (See fig19). We have found thatgrinding the samples by hand with a mortar and pestle (of corundum or sinteredalumina, not agate) gives us typical sums between 82-88% and that the results can benormalized to 98.5% (to match our target calibration standard SARM 9). Fig 17: Certified values for Chromite Standard SARM 9 Certified Values- As reported on C of AStandard Name Cr2O3 SiO2 FeO MgO Al2O3 CaO SUMSARM 9 46.45 0.61 24.96 10.85 15.17 0.16 98.20 Fig 18: Differences between chromite calibrations Chromite Sand Chrome calibration 2 Chrome calibration1 Cr2O3 45.308 41.697 SiO2 0.526 0.642 FeO 24.634 20.191 MgO 9.874 5.427 Al2O3 13.333 12.387 CaO 0.12 0.141 Sum: 93.795 80.485
Fig 19: Particle Size and XRF data on Hevi-Sand ground to varying fineness Amount retained (g) Screen Size Mesh #1 #2 #3 #4 #5 #6 106 µm No.140 7.32 6.4 4.59 2.69 2.69 1.73 75 µm No.200 1 1.44 1.33 1.4 2 1.76 53 µm No. 270 0.52 0.84 0.85 0.99 1.39 1.53 45 µm No. 325 0.25 0.5 0.52 0.58 0.82 1.05 20 µm No. 635 0.57 1.04 1.14 1.58 2.52 3.41 Pan Pan 0.48 1.11 1.01 1.06 1.53 1.06 total 10.14 11.33 9.44 8.3 10.95 10.54 % passing 200 mesh 17.95 30.80 37.29 50.72 57.17 66.89 XRF Data % Cr2O3 42.988 40.438 41.495 42.663 44.707 45.07 SiO2 0.958 1.913 1.493 1.325 0.572 0.626 FeO 23.748 22.264 22.778 23.538 24.753 24.964 MgO 9.618 9.983 9.556 9.718 9.83 9.895 Al2O3 12.841 12.793 13.408 13.313 14.132 14.341 CaO 0.111 0.111 0.105 0.101 0.092 0.092 Sum 90.264 87.502 88.835 90.658 94.086 94.988Inductively coupled Plasma (ICP) instruments are sometimes employed for chemicalanalysis of chromite as well; however this method requires complete digestion ofsolids into a liquid matrix for analysis, and this means very strong acid (usuallyHydrofluoric acid) heated under pressure to fully digest silica. This method can bemore time consuming and requires additional equipment and safety precautions due tothe issues handling such strong acid presents.ACID DEMAND / PHThese tests do seem to be pretty well under control although variations in proceduredo produce variations in results the deviation is very small. (see test proceduresappendix)LOISome foundries specify LOI values in there acceptance specs but have often notchecked it or the test method. If an uncontaminated chromite is tested in a oxidizingatmosphere there is a weight gain due to FeO becoming Fe2O3 and Fe3O4. If the testis carried out in a reducing atmosphere there should be no weight loss.It is therefore important to specify temperature / time and atmosphere to achieveconsistency of result. Fig 19a. shows a chromite sand tested in a Nitrogenenvironment on a TGA instrument (thermal gravimetric analysis), and Fig 19b: showsa chromite sand tested in air, note the oxidizing weight gain observed in air.
Fig 19a: TGA analysis in Nitrogen EnvironmentFig 19b: TGA in air (oxidizing environment)TurbidityThis is one of the most contentious tests and an area where there is little or nomeaningful interpretation of the results. Turbidity as it relates to chromite sand can bethought of as a measure of the light scattering caused by suspended particles in aliquid. The typical test method for most turbidity tests involves agitating chromitesand in water for a fixed amount of time and then allowing the heavy chrome sand tosettle for a fixed amount of time and measuring the resulting water for turbidity, thesuspended material in the water is generally thought to be low melting point silicateimpurities which are thought to contribute to certain types of casting defects (seepaper by J.D. Howden Chromite Double Skin Defect on Heavy-Section SteelCastings), so lower turbidity values are generally thought to be advantageous.
Most of the historical specifications for chromite sand define Turbidity inParts per Million (ppm) of silica. This is a reference to the Jackson Turbidity Test,which has been the industry standard for turbidity measurement for many years. Thistest uses a flat bottomed glass cylinder (known as a Jackson Tube, see fig 20.) with acandle flame placed approximately 10 cm (4 inches) from the bottom, liquid is pouredslowly into the tube while examining the flame down the cylinder and through theliquid. The tube is calibrated against solutions of diatomaceous earth (with silicapresent as silicic acid in the shells of the diatoms), a series of dilutions is typicallymade (1000, 500, 250 ppm) and added to the cylinder slowly. Designations are madeon the cylinder for each standard, based on the height of the cylinder each solutionreached to obscure the candle flame. This method of calibration is subject to theconsistency of the diatomaceous earth and of the care taken to calibrate and make thecorresponding designations on the cylinder. These measurements are sometimescalled Jackson Turbidity Units or JTUs . The use of the candle flame as the lightsource presented some drawbacks for analyzing samples with very fine suspendedparticles, color, and low turbidity. Modern instruments for turbidity measurementutilize a fixed light source, typically at a 90° angle from the light source, generallydecided to be best for detecting light scattering, which are generally referred to asNephlometers. Most modern instruments have adopted the Nephelometric TurbidityUnit or NTU as the preferred unit of measurement. The NTU, FTU, FAU are allequivalent as they are all based on the use of primary Formazin suspensions asturbidity standards, but do not correlate well to JTU measurements, some literaturecites ratios of 1 JTU= 4 NTU and others that cite 1JTU= 0.053 NTU ). Formazinstandards are highly reproducible and prepared from traceable consistent materials,and commercial standards are readily available. Depending on the intendedapplication modern electronic turbidity meters may employ additional detectors aswell to compensate for color, and particle size effects and to ensure increasedaccuracy over larger calibration ranges. For low level turbidity measurements ofdrinking waters a portable turbidity meter with only a 90° detector may be suitable,while higher turbidity samples (<100 NTU) may require dilution to be analyzed onthis instrument .Other instruments such as the Hach 2100 N turbidity meter utilize athree detector system (traditional 90° detector as well as a forward-scatter, andtransmitted light detector) which helps reduce the effects of color differences inturbidity measurements. This instrument is more suited to chromite turbidityapplications, and does not require dilution for samples under 4000 NTU, and is easyto standardize with readily available standards. (Figures 21 and 22 show a portableturbidity meter and a larger laboratory bench-top model).We believe that the industry should standardise on the NTU.
Fig 20: Jackson Turbidity Apparatus Figure 21: Portable Turbidity UnitFig 22: Laboratory Bench top model Turbidity Meter
As was mentioned previously the typical turbidity test for chromite, regardlessof the analytical method, involved agitation of dry chrome sand in water for a fixedamount of time in a effort to suspend the small particle sized tramp materialassociated with the chromite. A short amount of time is allowed to pass after agitationto allow the heavy solids to settle before the water is decanted and measured. Thetypical form of agitation of the chrome sand has been shaking the chrome and watertogether for 1 minute in a sealed jar by hand. What quickly becomes apparent withthis method is that the harder you shake the jar the higher the turbidity. It was seenthat “shake” test was very prone to variation due to differences in shaking velocitybetween users (see table 1 in appendix), with the same sample showing a range of 378to 739 NTU depending on the operator. Clearly there is a need to somehowstandardize this test to get accurate, reproducible results. Several alternative agitationmethods were investigated including magnetic stirring, horizontal shaking table, androtary devices. Another variable that influences turbidity results is agitation time, itwas seen that increased agitation time led to increased turbidity results regardless ofagitation method, and at 30 minutes of agitation time turbidity was still increasing. Itappears that the chromite is not being degraded and creating fines during the extendedagitation so it is assumed that the extended agitation is simply liberating more andmore finely sized material into suspension or perhaps breaking up the tramp materialincreasing the surface area of the suspended material and causing it to scatter morelight. The testing indicated that even what is considered good quality , low turbiditychromite sand could yield >1000 NTU turbidity values with extended mixing time.Since the goal was to create a reliable standardized method for turbidity measurementa familiar practical time of 1 minute agitation and 30 seconds settling time wasdecided upon. Additionally a wrist-action shaker was utilized to standardize thedifferences between individual user shaking velocities. The wrist action shaker provedto be the most advantageous method for reducing variability; it is designed to simulatethe human wrist movement, fully agitates the sample and provides reproducibleresults when used with a suitable turbidity meter (see Table 2 in appendix). The samesmall experiment was performed with individual operators using the wrist actionshaker instead of the traditional shake method and the results trend much closer toeach other. Our preferred method of analyzing turbidity in chrome sand is presentedin Appendix B-Methods and ProceduresSieve Analysis, Fines, AFS numberThese tests which on the face of it seem very simple and reproducible again turn outto be very contentious. This is really because no one really specifies clearly either thesieve type, sizes, or what they define as fines. Foundries often specify an AFS numberwhich is actually meaningless in its self, as many materials can meet this spec butfoundries would not necessarily be happy with the material supplied. Below are aseries of figures and tables (fig 23- 26) showing the scale of the potential differencesin reporting the same sample by different methods and a series of materials whichwould meet a foundries spec but which they would be unhappy with.The sieve analysis below is the same sample of sand put through British standardsieves and ASTM sieves; these combinations of sizes are typical of the sieves peopleuse in practice. In the right hand column are the micron sizes which match up withsome of the sieve numbers and not others. This coupled with the method of AFS
calculation, (i.e. % retained multiplied by the previous sieve number, then the calccolumn added together and divided by 100), leads to different AFS numbers whichcould possibly cause the material to be deemed out of specification from a foundriesperspective. Even more startling is the appearance of the sieve analysis chart, showinga double peak on the British standard sieves, compared to the more typical ASTMgraph, even though it is the same sand.If one analyses the differences one can see that over 92% of the material is between425 – 150 micron and that something around 70% is between 425 –and 212 micron.What appears to be a big difference at first glance is in fact irrelevant and is caused bythe majority of the crystals being very much the same size as the sieve apertures,therefore a very small change in aperture size results in a big change in the quantityretained. sieve size BS mesh ASTM US % Sieve Sieve micron retained No Calc %retained No Calc 2mm 8 0 10 0 1.7mm 10 0 12 0 1.4mm 12 0 14 0 1.18mm 14 0 16 0 1mm 0.5 16 6 18 0 850 18 0 0.9 20 14.4 710 1.2 22 19.2 25 0 600 25 0 3.1 30 62 500 2.3 30 50.6 35 0 425 35 0 19.6 40 588 355 33.6 44 1008 45 0 300 52 0 32.5 50 1300 250 27.2 60 1196.8 60 0 212 72 0 27.5 70 1375 180 85 0 80 0 150 31.6 100 2275.2 13 100 910 125 120 0 120 0 106 3.4 150 340 2.9 140 290 90 170 0 170 0 75 0.2 200 30 0.5 200 70 63 240 0 230 0 53 300 0 270 0 pan pan 0 pan 0 AFS AFS Total No Total No 100 49.3 100 46.1 Fig 23.The same sample using BS and ASTM sieves
If we take another example where foundries ask for a nominal 50% afs and less than1% fines on the pan, then they could be shipped the material below, ASTM US Sieve %retained No Calc 10 0 ASTM Mesh - Sieve Distribution 12 0 14 0 25 16 0 18 0 20 7 20 112 % Retained 15 25 0 10 25 30 500 35 0 5 15 40 450 0 45 0 10 14 18 25 35 45 60 80 120 170 230 9 50 360 Sieve No 60 0 8 70 400 80 0 Fig 26. 15 100 1050 120 0 20 140 2000The chart demonstrates that by foundries not defining 170 0accurately what they want they run the risk of getting 1 200 140something very undesirable that meets their 230 0specification. It is therefore clear that foundries should 270 0stop using AFS number as a shorthand, for sizing and pan 0 AFSmove to specifications which define grain size Total Nodistribution, 100 50.1Discussion of Chromites beneficial properties, in relation to foundries, realrequirements.In order to decide on what properties truly matter to foundries it is important toconsider the effects of each of the test parameters and the practical disadvantages ofdeviation from the results. Therefore in reviewing these effects one must considerwhat foundries are trying to achieve by using chrome sand. 1. Rapid Heat abstraction rate. 2. Good permeability reducing gas pressures and overheating. 3. Low thermal expansion, dimensional stability, no veining. 4. High resistance to penetration and burn on, improved Surface finish. 5. Lower binder and catalyst additions and thus lower gas evolution.
As can be seen from the above the desirable properties fall into two key areas 1-4,the physical properties of the materials and 5 the effect of these properties onbinder usage.Properties (1-4)In the authors opinion it is very difficult to make hard and fast rules in foundriesas a lot of the data on which foundry practice is based is either extrapolated graphs(where products or effects cannot be tested at casting temperatures), or based onthe conclusions of foundries practical experience.This results in a need for foundries to develop a philosophy which overcomes thelack of cold hard facts. If at its simplest we say that in an ideal world wheremelting, pouring, and moulding is perfect, then if ingate velocity, pouring andsolidification time are all zero, then there would be no time to generate defects.Unfortunately of course this is impossible, but it does at least allow us to concludethat, everything that moves in the opposite direction is undesirable.Given these objectives by making a mould with chromite sand rather than silicasand we can expect due to its higher density, specific heat and conductivity, thatthe immediate solidified skin which is created during mould filling will be thickerthis also means it has a greater resistance to being re-melted during mould fillingand being washed away, which in turn infers that the mould can be filled morequickly, this in turn, given chromite sands low thermal expansion characteristics,results in less chance of veining, erosion, spalling, and dimensional problems.Likewise this rapid heat abstraction and solidified skin formation, reduces theincidence of penetration and Burn on.As the above clearly drives us towards our simplistic goals, we concluded thatmaximising the bulk density of the material should result in significant technicaladvantages. The only downside in maximising bulk density is the reduction inpermeability. (We will do some more testing on this once our new plant isoperational. This will show how sieve analysis, afs no, bulk density andpermeability are interrelated.) We have therefore decided that we should create anumber of tailor made Hevi-Sand specifications aimed at allowing foundries tomaximise bulk density for an acceptable reduction in permeabilityGas evolution and resin usageSimilarly, in the next stage of testing we will analyse the test data for HS processsand, a typical foundry chromite, and the various samples of HS.We expect to find from this testing that as you move existing chromite sand froma 2 sieve sand to a 4/5 sieve sand, not only does the bulk density increase and thepermeability drop, it also reduces the resin requirement even though the calculatedsand surface area has increased, the reason for this is that the improvedcompaction reduces the size of the voids in the compacted sand and in turnincrease the number of contact points with other sand grains hence a stronger sandfor less binder. While this means lower binder usage and less gas evolution duringcasting, it must be remembered that if the sand mass is denser then there is moreresin for a given volume of sand. We therefore intend to include an adjustmentfor the effect of density on the resin content.
CONCLUSIONSThe HS process project, and the associated research and testing has thrown up anumber of issues with regard to the supply and procurement process which currentlyexists in the industry. 1. There is no definitive or agreed world standard specification for foundry quality chromite sand. 2. Test procedures and technical requirements are often inconsistent or based on habit / past experience or in many instances based on information and products which were defined 50 years ago. 3. There are significant casting benefits to be gained by creating a range of tailor made Hevi-Sand products which are specific to the casting being produced in any given foundry. This can be about maximising bulk density to increase heat abstraction, maximising permeability to reduce gas pressure, maximising fineness to improve cosmetic surface finish, or working with foundries to create the best most cost effective “jack of all trades” for there foundry.We hope that the information and the arguments we have outlined in this paper can beused by the industry and its technical institutions to review recommended acceptancespecifications.We believe the table below should be the minimum requirements, while as a supplierwe can also make suggestions for product enhancement. Our recommended testprocedures are attached as appendices. Should you wish to see the detailed studiesplease contact Amcol.HEVI-SAND Recommended Foundry Minimum SpecificationPhysical analysis Chemical analysisGrain size distribution To Suit Foundry Cr > 47.5%PH 6.8 – 7.3 Fe203 < 27.5%Turbidity < 200 NTU Silicates < 0.65%LOI (in nitrogen) < 0.1% Ca < 0.2%Acid demand Ph3 5ml, Ph4 3ml, Ph5 2ml.
Appendix A- Data Table 1: Data for “Shake” Test Turbidity method Average Operator # Turbidity (NTU) #1 518 #2 445 #3 378 #4 584 #5 496 #6 427 #7 739 #8 595 #9 412 #10 616 #11 454 #12 415 Average Results 507 Standard Deviation 107.3Different individuals in the Hoffman Estates Lab tested the sample with the sameprocedure, and equipment. There is variability in these results, the lowest result seenwas 378 NTU and the highest was 739 NTU, the average results is nearly 100 NT lessthan the average reported in table 1. Table 8: General Data for Turbidity method utilizing Wrist Action Shaker Average Operator # Turbidity (NTU) #1 465 #2 471 #3 478 #4 434 #5 446 #6 452 #7 456 #8 512 #9 451 #10 459 #11 470 #12 438 Average Results 461 Standard Deviation 20.8As done previously in table 2, individual users were asked to run the turbidity method again using the wrist actionshaker, instead of shaking by hand, it is apparent that the distribution of results is much narrower and the standarddeviation is better using this method.
Appendix B- Methods and ProceduresMeasurement of Turbidity of Chrome Sand-Equipment:500 ml Pyrex Erlenmeyer FlaskHach 2100N laboratory Turbidity Meter, calibrated with Hach Stab Cal standardsolutions of 0, 20, 200, 1000 and 4000 NTU as per manufacturers instructions.Instrument should be recalibrated quarterly.Burell – Wrist Action Shaker ( amplitude lever set to 10 )Turbidity Free water (Distilled/ De-ionized Water)Drying ovenScale- Capable of accurately measuring at least 250 grams 1. Dry a sufficient amount of chrome sand to a constant weight in a drying oven (110 C) 2. Weigh 100g dry chrome sand in a weigh boat and add to 500 ml Flask 3. Weigh 250 grams distilled water into a beaker and add to 500 ml Flask 4. Place Flask into Grip of Wrist Action Shaker and tighten until secure (do not over tighten or risk cracking the neck of the flask) and shake for 1 minute on maximum amplitude (separate lever on side on shaker, set to “10”). 5. After shaking 1 minute, allow fleaker to stand for 30 seconds, after settling seconds pour off turbid water into beaker. 6. Carefully pour water from beaker into clean, dry 30 ml Hach sample vial, secure cap 7. wipe vial with cloth, apply silicone oil to vials as necessary, and insert into Hach 8. Make sure ratio and signal averaging modes are active (lights will be green on these keys), and make sure the units are NTU 9. Record first value displayed by Hach, as the numbers fluctuate due to settling while in instrument C:Documents andSettingsJoeMy DocumentseildonrefractoriesChromiteChromite Double Skin Defects Paper.DOCDouble skin defect hevi-sand ppt